Photonic Band Gap Crystals. Srivatsan Balasubramanian. Summary. Physics of photonic bandgap crystals. Photonic Crystals Classification. Fabrication. Applications. Protoype photonic band gap devices. Current Research. Future Directions. Conclusion. What is a PBG ?.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
This will revolutionize photonics the way transistors revolutionized electronics.
PBG formation can be regarded as the synergetic interplay between two distinct resonance scattering mechanisms. The first is the “macroscopic” Bragg resonance from a periodic array of scatterers. This leads to electromagnetic stop gaps when the wave propagates in the direction of periodic modulation when an integer number, m=1,2,3…, of half wavelengths coincides with the lattice spacing, L, of the dielectric microstructure. The second is a “microscopic” scattering resonance from a single unit cell of the material. In the illustration, this (maximum backscattering) occurs when precisely one quarter of the wavelength coincides with the diameter, 2a, of a single dielectric well of refractive index n. PBG formation is enhanced by choosing the materials parameters a, L, and n such that both the macroscopic and microscopic resonances occur at the same frequency.
These conditions on the geometry, scattering strength, and
the purity of the dielectric material severely restrict the set of
engineered dielectrics that exhibit a PBG.
Materials used for making a PBG:
Simple examples of one-, two-, and three-dimensional photonic crystals. The different colors represent materials with different dielectric constants. The defining feature of a photonic crystal is the periodicity of dielectric material along one or more axes. Each of these classifications will be discussed in turn in the following slides.
The multilayer thin film show above is a one-dimensional photonic crystal. The term “one-dimensional” refers to the fact that the dielectric is only periodic in one direction. It consists of alternating layers of materials (blue and green) with different dielectric constants, spaced by a distance a. The photonic band gap exhibited by this material increases as the dielectric contrast increases.
The photonic band structures for on-axis propagation shown for three different multilayer films, all of which have layers of width 0.5a.
Left: Each layer has the same dielectric constant. ε = 13. Center: Layers alternate between ε = 13 and ε = 12.
Right: Layers alternate between ε = 13 and ε = 1.
It is observed that the photonic gap becomes larger as the dielectric contrast increases.
(2) The reflected waves are in phase and reinforce one another.
(3) They combine with the incident wave to produce a standing wave that
does not travel through the material.
(1) A wavelength outside the band gap enters the 1D material.
(2) The reflected waves are out of phase and cancel out one another.
(3) The light propagates through the material only slightly attenuated.
Left: A periodic array of dielectric cylinders in air forming a two-dimensional band gap.
Right: Transmission spectrum of this periodic lattice. A full 2D band gap is observed in the wavelength range 0.22 microns to 0.38 microns.
Left: A defect is introduced into the system by removing one of the cylinders. This will lead to localization of a mode in the gap at the defect site
Right: It is seen that some transmission peak is observed in the forbidden band. This corresponds to the defect state which leads to spatial localization of light and has useful applications in making a resonant cavity.
A two dimensional photonic crystal with two 60o bends, proposed by Susumu Noda’s group. These structures are easy to fabricate but they have the problem of the photons not being confined on the top and bottom. By introducing point defects like making a hole larger or smaller than the normal size, the slab can be made to act like a microcavity and can be used for making optical add-drop filters.
(1) For a two-dimensional band gap, each unit cell of the structure produces reflected waves.
(2) Reflected and refracted waves combine to cancel out the incoming wave.
(3) This should happen in all possible directions for a full 2D bandgap.
3D photonic bandgaps are observed in
The inverted diamond structure was one of the first prototype structures predicted by Chan and Soukoulis to exhibit a large and robust 3D PBG. It consists of an overlapping array of air spheres arranged in a diamond lattice. This structure can be mimicked by drilling an array of criss-crossing cylindrical holes in a bulk dielectric. The solid backbone consists of a high refractive index material such as silicon leading to a 3D PBG as large as 27% of the center frequency. The minimum refractive index of the backbone for the emergence of a PBG is 2.0
This is first three dimensional photonic crystal to be made and it was named Yablonovite after Yablonovitch who conceptualized it. A slab of material is covered by a mask consisting of triangular array of holes. Each hole is drilled through three times, at an angle 35.26 away from normal, and spread out 120 on the azimuth. The resulting criss-cross holes below the surface of the slab produces a full three dimensional FCC structure. The drilling can be done by a real drill bit for microwave work, or by reactive ion etching to create a FCC structure at optical wavelengths. The dark shaded band on the right denotes the totally forbidden gap
The “woodpile” structure, suggested by Susumu Noda’s group, represents a three-dimensional PBG material that lends itself to layer-by-layer fabrication.It resembles a criss-crossed stack of wooden logs, where in each layer the logs are in parallel orientation to each other. To fabricate one layer of the stack, a SiO2-layer is grown on a substrate wafer, then patterned and etched. Next, the resulting trenches are filled with a high-index material such as silicon or GaAs and the surface of the wafer is polished in order to allow the next SiO2 layer to be grown. The logs of second nearest layers are displaced midway between the logs of the original layer. As a consequence, 4 layers are necessary to obtain one unit cell in the stacking direction. In a final step, the SiO2 is removed through a selective etching process leaving behind the high-index logs.
SEM picture of a cross-section along the cubic (110) direction of a Si inverse opal with complete 5% PBG around 1.5 um. The structure has been obtained through infiltration of an artificial opal with silicon (light shaded regions) and subsequent removal of SiO2 spheres of the opal. The air sphere diameter is 870 nanometers. Clearly visible is the complete infiltration (diamond shaped voids between spheres) and the effect of sintering the artificial opal prior to infiltration ( small holes connecting adjacent spheres.)
Computer rendering of a three dimensional photonic crystal, put forth by Joannopoulos and his group, showing several horizontal periods and one vertical period consisting of a FCC lattice of air holes (radius 0.293a, height 0.93a) in dielectric. This allows one to leverage the large body of analyses, experiments, and understanding of those simpler structures. This structure has a 21% gap for a dielectric constant of 12.
The tetragonal lattice of square spiral posts exhibits a complete 3D PBG and can be synthesized using glancing angle deposition (GLAD) method. This chiral structure, suggested by John and Toader, consists of slightly overlapping square spiral posts grown on a 2D substrate that is initially seeded with a square lattice of growth centers. Computer controlled motion of the substrate leads to spiraling growth of posts. A large and robust PBG emerges between the 4th and 5th bands of photon dispersion. The inverse structure consisting of air posts in a solid background exhibits a even larger 3D PBG.
The scaffolding structure (for it’s similarity to a scaffolding) is a rare example of a photonic crystal that has a very different underlying symmetry from the diamond structure yet has a photonic band gap. The band gap is small but definitely forbidden and this was suggested by Joseph Haus and his colleagues.
A marriage of liquid and photonic crystals as conceptualized by Busch and John. An inverse opal photonic crystal structure partially infiltrated with liquid crystal molecules. Electro-optic tuning can cause the bandgap to wink in and out of existence. This can have disruptive influence on our present technologies as will be discussed later.
PCFs come in two forms:
Internal Reflection (M-TIR) principle
Architectures for 2D photonic crystal micro-lasers are shown above. (a) The Band Edge
microlaser utilizes the unique feedback and memory effects associated with a photonic band
edge and stimulated emission (arising from electron-hole recombination) from the multiple
quantum well active region occurs preferentially at the band edge. There is no defect mode
Engineered in the 2D PBG. (courtesy of S. Noda, Kyoto University). (b) Defect Mode micro
laser requires the engineering of a localized state of light within the 2D PBG. This is created
through a missing pore in the 2D photonic crystal. Stimulated emission from the multiple
quantum well active region occurs preferentially into the localized mode. (courtesy of Axel
Scherer, California Institute of Technology).
Add-drop filter for a dense wavelength division multiplexed optical communication system. Multiple streams of data carried at different frequencies F1, F2, etc. (yellow) enter the optical micro-chip from an external optical fiber and are carried through a wave guide channel (missing row of pores). Data streams at frequency F1 (red) and F2 (green) tunnel into localized defect modes and are routed to different destinations. The frequency of the drop filter is defined by the defect pore diameter which is different from the pore diameter of the background photonic crystal.
An artist’s conception of a 3D PBG woodpile structure into which a micro-laser
array and de-multiplexing (DEMUX) circuit have been integrated. (courtesy of S.
Noda, Kyoto University, Japan). These photonic integrated circuits will be prime
movers for deeper penetration of optical networking into telecommunications.
Micro-photonic all-optical transistor may consist of an active region buried in the intersection of two wave-guide channels in a 3D PBG material. The two-level systems (“atoms”) in the active region are coherently pumped and controlled by laser beams passing through the wave guides. In addition, the 3D PBG material is chosen to exhibit an abrupt variation in the photon density of states near the transition frequency of the atoms. This leads to atomic “population inversion” through coherent pumping, an effect which is forbidden in ordinary vacuum. The inversion threshold is characterized by a narrow region of large differential optical gain (solid curve in the inset). A second, “control laser” allows the device to pass through this threshold region leading to strong amplification of the output signal. In ordinary vacuum, population inversion is unattainable (dashed curve in the inset).
Artist’s depiction of an electro-actively tunable PBG routing device. Here the PBG material has been infiltrated with an optically anisotropic material (such as a liquid crystal) exhibiting a large electro-optic response. When a voltage is applied to the electro optically tunable PBG, the polarization state (yellow arrows) can be rotated, leading to corresponding shifts in the photonic band structure. This allows light from an optical fiber to be routed into one of several output fibers.
With optical integrated circuits and optical transistor technology being rendered possible by photonic crystals, quantum computing with localized light is a very promising technology for the future. Immense parallelism, unprecedented speeds, superior storage density, minimal crosstalk and interference are some of the advantages that one gets while migrating towards optical computing.
An artistic view of a collage of different photonic crystal devices going into an integrated circuit. The buildings are 3-D PBG crystals. The clear buildings with the blue balls depict a metallo-dielectric structure. The green "forests" show two-dimensionally periodic photonic crystals. The red "roads" with holes in them are one-dimensionally periodic crystals.
1. Yablonovitch, E. Phys. Rev. Lett. 58, 2059–2062 (1987).
2. John, S. Phys. Rev. Lett. 58, 2486–2489 (1987).
3. Ho, K. M., Chan, C. T. & Soukoulis, C. M. Phys. Rev. Lett. 65, 3152–
4. Yablonovitch, E., Gmitter, T. J. & Leung, K. M. Phys. Rev. Lett.
67, 2295–2298 (1991).
5. Sozuer, H. S., Haus, J. W. & Inguva, R. Phys. Rev. B 45, 13962–13972
6. Busch, K. & John, S. Phys. Rev. Lett. 83, 967–970 (1999).
7. Yablonovitch, E, Nature 401, 540-541 (1999)
8. John.S, Encyclopedia of Science and Technology, Academic